Cellulose/polyvinyl alcohol based hydrogels for reconfigurable lens T. Jayaramudua, Hyun-U Koa, Xiaoyuan Gaoa, Yaguang Lia, Sang Yeon Kimb, Jaehwan Kim*a a Center for NanoCellulose Future Composites, Department of Mechanical Engineering, Inha University, 100, Inha-ro, Nam-gu, Incheon, South Korea; b Interaction Laboratory of Advanced Technology Research Center, Korea University of Technology and Education, 1600, Chungjeol-ro, Byeongcheon-myeon, Dongnam-gu, Cheonan-si, Chungcheongnam-do, South Korea
ABSTRACT Electroactive hydrogels are attractive for soft robotics and reconfigurable lens applications. Here we describe the design and fabrication of cellulose-poly vinyl alcohol based hydrogels. The fabricated hydrogels were confirmed by Fourier transformer spectroscopy, swelling studies, thermal analysis, surface morphology of fabricated hydrogel was study by using scanning electron microscopy. The effect of poly vinyl alcohol concentration on the optical and electrical behavior of hydrogels was studied. Key words: Polyvinyl alcohol, Cellulose, Dimethylacetamide, Electroactive hydrogel.
1. INTRODUCTION During the past few decades hydrogels have received great consideration in numerous applications such as biomedical, tissue engineering, drug delivery, bioactive electrode coatings actuators biomimetic field.1,2,3,4 Electroactive hydrogels are much interested in soft robotic applications due to soft and flexible properties and these materials exhibit bending/longitudinal deformation by applying low voltages.5 Generally hydrogels are hydrophilic three dimensional network structures which are formed either physical or chemical crosslinking by using the synthetic or natural materials.6 Electroactive hydrogels are prepared by adding various electrical nature materials, for example, conducting metal nanoparticles, electrically conductive polymer nanoparticles and electroactive polymers in the preparation of electroactive hydrogels network.7,8,9 Among them, we choose Poly vinyl alcohol (PVA) and cellulose for preparation of electroactive hydrogels. In general, these materials have electroactive nature. 10,11 Cellulose is one of the most abundant natural resource organic material in nature. Now a days, cellulosed based materials are considered for large number of applications due to the advantages, such as biodegradability, biocompatibility, low cost, mechanical, readily availability and chemical structure.12,13,14 Based on these properties and applications of cellulose, its derivatives and combination of other synthetic or natural materials are used for various fields. Recently cellulose with PVA based hydrogels were prepared science cellulose have large amount of hydroxyl groups and these groups can easily react with hydroxyl groups of PVA so as to form intermolecular hydrogen bond.15 The aim of this study is to enhance the deformation of PVA based electroactive hydrogels by physical blending PVA with cellulose. The fabricated hydrogels network structure was confirmed from FTIR, TGA, studies and the transparency was measured using UV-vis spectroscopy. The actuation performance test was carried out by using AC voltage.
; Tel: +82-32-831-7325; Fax: +82-32-832-7325, ncfc.inha.ac.kr
2. MATERIALS AND METHODS 2.1 Materials Cotton pulp (MVE, DP-4580) was supplied by Buckeye Technologies Co. Ltd. (USA) and Poly vinyl alcohol (PVA = 89 000-98 000 g mole-1, 99% hydrolyzed). Extra pure lithium chloride (LiCl) was carefully dried by using an oven at 110 oC, 2 h before use, N,N-dimethylacetamide (DMAc) were purchased from Sigma-Aldrich. The DI water was used throughout experiment. 2.2 Preparation of PVA-cellulose hydrogel Cellulose/PVA (CP) hydrogels were prepared by blending method. Before blending cellulose and PVA solutions were prepared. Here a common solvent was used for both solution preparations. Preparation of the cellulose solution was described in our previous paper16 and here is brief explanation. The pure cotton pulp was dispersed in 8.5 % LiCl/DMAc solvent and stirred by using magnetic stirrer at room temperature over a period of 5 days after that completion of this process obtained 1.5 wt % of cellulose solution and also 1.5 wt% of PVA solution was obtained by above similar process at 60 OC. After getting the both solutions were mixed with different ratios 75/25, 50/50 and 25/75, stirred at room temperature until homogeneous mixture getting after that the solution was poured in Petridis and kept in oven at 30OC for a period of 3 days. After 3 days transparent hydrogel is formed and the formed hydrogel was immersed in 500 mL beaker containing 250 mL of DI water. The water was repeatedly changed every 6 h up to 5 days to remove LiCl/DMAC and unreacted materials from the hydrogel. 2.3 Characterization of PVA- Cellulose hydrogels The FTIR spectra were used to study the formation of CP hydrogel. Before, analysis of the FTIR spectra the samples were completely dried in the oven at 60 OC for 6 h and the samples were examined between 500-4000 cm-1 on Bruker Optics, Billerica, MA using the KBr pellet method. Transparency analysis of the CP hydrogels was performed by using UV-visible spectroscopy (HP8452A, Agilent). The hydrogels were cut into a desire shape for transparency measurement and the spectra recorded from 200-800 nm. The thermal behavior of the Cellulose and CP hydrogels were studied by thermogravimetric analysis (TGA) (NETZSCH, STA 409 PC), at a heating rate of 10 OC/min under a constant nitrogen flow (20mL/min). 2.4 Actuation test The actuation test was carried out by using a laser displacement sensor (Keyance LK-G85, Tokyo, Japan) a high voltage amplifier connected to a function generator, (33220A, Agilent), Lab view software on a personal computer. Before conducting the actuation test the desired shape of the hydrogels (10 x 10 x 0.4 mm) were equilibrated in DI water for 24 h after reaching of equilibration, the swollen hydrogels were kept in between two electrodes (polyimide tape attached on ITO glass) and an electric field was applied between two electrodes. Displacement of the hydrogel was measure by the laser displacement sensor along with a data acquisition system (PULSE, B&K) as shown in Fig.1. Pulse analyser
Laser DopplerVibrometer (LDV)
Ito Barr (Indium tin oxide I
Sample: 10%10 X 0.4mm
High voltage amplifier
Figure 1. Schematic setup of actuation test.
3. RESULTS & DISCUSSION The cellulose/PVA (CP hydrogel) hydrogels were developed by physical blending method and in this method PVA react with cellulose by intermolecular interaction so as to form transparent hydrogels. Fig. 2 shows the schematic formation of the hydrogels. The formation of the hydrogels are confirmed from FTIR spectra (Fig.3)
Figure 2. Schematic diagram of CP hydrogels formation
3.1 Fourier transform Infrared Spectroscopy The FTIR spectra of the PVA, cellulose and CP hydrogels are showed in Fig.3. From Fig. 3, the CP hydrogels show the similar peaks of PVA, which demonstrates that the cellulose is uniformly dispersed in PVA. The characteristic peaks at 1098 cm-1 and 2923 cm-1 are related to stretching vibrations of the C-O and C-H. A broad absorption peak at 3438 cm-1 corresponds to the –OH stretching vibration of PVA. While these peaks were slightly shifted to 1098 cm-1 and 2923 to 1063cm-1 and 2917 cm-1 in CP hydrogel and also the -OH group was slightly shifted from 3438 cm-1 to 3425 cm-1 in CP hydrogel. The intensity of this peak was slightly decreased and appeared to be a bit broader than the –OH of the PVA. This is due to the strong intermolecular bond formation between the PVA and cellulose matrix.17 An interestingly absorption peak was absorbed at 899 cm-1 this the b-glucan group of the cellulose and also the fingerprint region peaks intensity increased due to the crystalline structure of the cellulose.18,19,20 The pure cellulose hydrogel shows the above characteristic peaks of the CP hydrogel peaks with slightly changes (3427 cm-1, 2920 cm-1, 1069 cm-1 and 896 cm-1). 100
-cellulose hydrogel - PVA hydrogel - CP hydrogel 60 4000
Wavenumber (cm 1) Figure 3. FTIR spectra of PVA, Cellulose and CP hydrogels
3.2 UV-Vis transmittance The prepared CP hydrogel transparency was measured by using UV-vis spectroscopy. The transparency depends on the concentration of PVA in the prepared hydrogels. Figure 4 shows the transparency of the CP hydrogel. The transparency was decreased with increasing the PVA concentration in the hydrogel and also it depends on the thickness of the hydrogel. As increasing the thickness of the hydrogel the transmittance decreases. However the overall transparency was followed in the sequence of CP75